The Use of Polarizable [AuX2(CN)2]- (X = Br, I) Building Blocks Toward the Formation of Birefringent Coordination Polymers
Jeffrey S. Ovens; Andrew R. Geisheimer; Alexei A. Bokov; Zuo-Guang Ye; Daniel B. Leznoff; Inorganic Chemistry 49 (2010) 9609–9616; doi:10.1021/ic101357y

data_4316831
_publ_contact_author_address
; 
Leznoff, Daniel B.
Department of Chemistry
Simon Fraser University
Burnaby, British Columbia
Canada         V5A 1S6
;
_publ_contact_author_email       dleznoff@sfu.ca
_publ_contact_author_fax         +1-778-782-3765
_publ_contact_author_name        'Daniel B. Leznoff'
_publ_contact_author_phone       +1-778-782-4887
_publ_section_title
;
 The Use of Polarizable [AuX2(CN)2]- (X = Br, I) Building Blocks Toward
 the Formation of Birefringent Coordination Polymers
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9609
_journal_page_last               9616
_journal_paper_doi               10.1021/ic101357y
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'C18 H36 Au1 I2 N3'
_chemical_formula_sum            'C18 H36 Au I2 N3'
_chemical_formula_weight         745.28
_chemical_name_systematic        ?
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_cell_angle_alpha                90
_cell_angle_beta                 116.446(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.363(3)
_cell_length_b                   17.918(4)
_cell_length_c                   13.020(3)
_cell_measurement_reflns_used    6473
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.72
_cell_measurement_theta_min      2.16
_cell_volume                     2582.4(10)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution
; 
SIR92 (Altomare et al, 1994)
CRYSTALS (Watkin, 1988) 
;
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.914
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.064
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            15127
_diffrn_reflns_theta_full        26.435
_diffrn_reflns_theta_max         28.424
_diffrn_reflns_theta_min         1.890
_exptl_absorpt_coefficient_mu    8.093
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3321
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            orange-red
_exptl_crystal_density_diffrn    1.917
_exptl_crystal_description       plate
_exptl_crystal_F_000             1400
_exptl_crystal_size_max          0.36
_exptl_crystal_size_mid          0.35
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.54
_refine_diff_density_min         -1.08
_refine_ls_extinction_method     None
_refine_ls_goodness_of_fit_ref   1.1494
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         2903
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1132
_refine_ls_R_factor_gt           0.0545
_refine_ls_shift/su_max          0.0012751
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[\s^2^(F) + ( 0.02P)^2^ + 0.10P] 
 ,where P=(max(Fo,0) + 2Fc)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1025
_refine_ls_wR_factor_gt          0.0687
_refine_ls_wR_factor_ref         0.0671
_reflns_limit_h_max              14
_reflns_limit_h_min              -16
_reflns_limit_k_max              24
_reflns_limit_k_min              0
_reflns_limit_l_max              17
_reflns_limit_l_min              0
_reflns_number_gt                3070
_reflns_number_total             5937
_reflns_threshold_expression     I>2.0\s(I)
_oxford_diffrn_Wilson_B_factor   4.47
_oxford_diffrn_Wilson_scale      376.83
_oxford_refine_ls_r_factor_ref   0.0518
_oxford_refine_ls_scale          0.06140(15)
_oxford_reflns_number_all        5937
_oxford_reflns_threshold_expression_ref I>2.5\s(I)
_cod_data_source_file            ic101357y_si_001_3.cif
_cod_data_source_block           diIodo
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_formula_sum        'C18 H36 Au1 I2 N3'
_cod_database_code               4316831